Gass Ionomer Cement
Click here to load reader
Embed Size (px)
Transcript of Gass Ionomer Cement
- 1.GLASS IONOMERCEMENT dr shabeel pn
2. INTRODUCTION Glass ionomer cement is a tooth coloured material, introduced by Wilson &Kent in 1972.Material was based on reaction between silicate glass powder & polyacrylic acid.They bond chemically to tooth structure & release fluoridefor relatively long period. 3. CLASSIFICATION
- For luting
- For restoration
- III.For liner & bases
- IV.Fissure & sealent
- V.As Orthodontic cement
- VI.For core build up
Type II.1Restorative esthetic Type II.2Restorative reinforced Type Type Type Type Type Type 4. COMPOSITION
- Powder :-
- Acid soluble calcium fluroalumino silicate glass.
- Silica- 41.9%
- Aluminum fluoride-1.6%
- Calcium fluoride- 15.7%
- Sodium fluoride-9.3%
- Aluminum phosphate- 3.8%
- Fluoride portion act as ceramic flux. Strontium,
- Barium or zinc oxide provide radio opacity.
- Liquid :-
- 1.Polyacrylic acid in the form co-polymer with itaconic acid & malice acid .
- 2. Tartaric acid : improves handling characteristic
- & increase working time.
- 3. Water: Medium of reaction & hydrates the
- reaction products
6. SETTING REACTION
- When the powder & liquid are mixed, Surface of glass particles are attacked by acid. then Ca, Al, sodium, & fluoride ions are leached into aqueous medium.
- Calcium poly salts are formed first, then followed by aluminum poly saltswhich cross link with poly anion chain.
- Set cement consist of unreacted powder particle surrounded by silica gel in amorphous matrix of hydrated calcium & aluminum poly salts.
- Calcium poly salts are responsible for initial set.
- Aluminum poly salts form the dominant phase.
- Water plays an important role in structure of cement.
- After hardening, fresh cement is extremely prone to the cracking & crazing, due to drying of loosely bound water .
- Hence these cements must be protected by application of varnish.
9. SETTING TIME
- Type I4 - 5 minutes
- Type II7 minutes
- Compressive strength - 150 mpa
- Tensile strength-6.6 mpa.
- Hardness-49 KHN.
11. Solubility & Disintegration:-
- Initial solubility is high due to leaching of intermediate products.
- The complete setting reaction takes place in 24 hrs, cement should be protected from saliva during this period.
- Adhesion :-
- Glass ionomer cement bonds chemically to the tooth structure.
- Bonding is due to reaction occur between carboxyl group of poly acid & calcium of hydroxyl apatite.
- Bonding with enamel is higher than that of dentin ,due to greater inorganic content.
- Esthetics :-
- GIC is tooth coloured material & available in different
- Inferior to composites.
- They lack translucency & rough surface texture.
- Potential for discolouration & staining.
- Biocompatibilty :-
- Pulpal response to glass ionomer cement is favorable.
- Pulpal response is mild due to
- - High buffering capacity of hydroxy apatite.
- - Large molecular weight of the polyacrylic
- acid ,which prevents entry into dentinal tubules.
- Anticariogenic properties :-
- Fluoride is released from glass ionomer at the time of mixing & lies with in matrix. Fluoride can be released out without affecting the physical properties of cement.
- Initial release is high. Butdeclines after 3 months.
- After this, fluoride release continuous for a long period.
- Fluoride can also be taken up into the cement duringtopical fluoride treatment and released again ,thus GIC act asfluoride reservoir.
- 1 .Preparation of tooth surface :-
- The enamel & dentin are first cleaned with pumice slurry followed by swabbing with polyacrylic acid for 5 sec. After conditioning & rinsing ,tooth surface should isolate & dry.
- 2. Proportioning & mixing :-
- Powder & liquid ratio is 3:1 bywt. Powder & liquid is dispensed just prior to mixing.
- First increment is incorporated rapidly to producea homogenous milky consistency.
- Mixing done in folding method to preserves gel structure.
- Finished mix should have a glossy surface.
- 3.Protection of cement during setting :-
- Glass ionomer cement is extremely sensitive to air & water during setting.
- Immediately after placement into cavity, preshaped matrix is applied to it.
- 4.Finishing :-
- Excess material should be trimmed from margins.
- Hand instruments are preferred to rotary tools to avoid ditching.
- Further finishing is done after 24hrs.
- 5. Protection of cement after setting :-
- Before dismissing the patient ,restoration is again coated with the protective agent to protect trimmed area.
- Failure to protect for first 24hrs results in weaken cement.
- Inherent adhesion to the tooth surface.
- Good marginal seal.
- Anticariogenic property.
- Minimal cavity preparation required.
- Disadvantages :-
- Low fracture resistance.
- Low wear resistance.
- Water sensitive during setting phase .
- Less esthetic compared to composite.
- Uses :-
- Anterior esthetic restoration material for class III & V restorations.
- For luting.
- For core build up.
- For eroded area .
- For atraumatic restorative treatment.
- As an orthodontic bracket adhesive.
- As restoration for deciduous teeth.
- Used in lamination/ Sandwich technique.
20. SANDWICH TECHNIQUE
- Devolped by Mclean,
- To combine the beneficial properties of GIC & composite.
- Clinical steps:-
- After cavity preparation,
- condition the cavity to develop good adhesion with GIC.
- Place Type III GIC into prepared cavity.
- After setting, etch the enamel & GIC with orthophosphoric acid for 15 seconds.
- This will improvemicromechanical bondto composite resin.
- Apply a thin layer of low viscosity enamel bonding agent & finally place the composite resin over GIC & light cure it.
- Polymerisation shrinkage is less,due to reduced bulk of composite.
- Favorable pulpal response.
- Chemical bond to the tooth.
- Anticariogenic property.
- Better strength,finishing,esthetics of overlying composite resin.
- 1. Water settable glass ionomer cement :-
- Liquid is delivered in a freeze dried form ,which is incorporated into the powder.
- Liquid used is clean water.
- 2.Resin modified glass ionomer cement:-
- Powder component consist of ion leachable fluroalumino silicate glass particles & initator for light curing.
- Liquid component consist of water & poly acrylic acid with methacrylate & hydroxyl ethyl methacrylate monomer.
- 3 .Metal modified glass ionomer cement :-
- Glass ionomer have been modified by addition of filler particles ,to improve strength ,fracture toughness & resistance to wear.
- Silver alloy admix / miracle mix:-
- This is made by mixing of spherical silver amalgam alloy powder with glass ionomer powder.
- Bonding of silver particles to glass ionomer particles by fusion through high temperature sintering.
- 4. Compomer:-
- Compomer is a composite resin that uses an ionomer glass which is the major component of glass ionomer as the filler.
- Small quantity of dehydrated polyalkenoic acid incorporated with filler particles,
- Setting reaction is light activated.
- Adhesive system used with compomer is based on acid etch found with all composite resin.
26. THANK YOU